# Modeling the strain-rate dependence of fatigue life of hot-pressed silicon nitride

**Modeling the strain-rate dependence of fatigue life of hotpressed silicon nitride Vinod Sharma, S. Nemat-Nasser *, Kenneth S. Vecchio Center of Excellence for Advanced Materials, Department of AMES, 9500 Gilman Drive, University of California, San Diego, La Jolla, CA 92093-0416, USA Received 22 March 1997; revised version received 5 March 1998 Abstract This paper presents the results of a micromechanical model used to explain the strain-rate dependence of the compression fatigue lives of amorphous and crystalline grain boundary phase; denoted by ABP and CBP silicon nitrides, respectively. When the strain-rate is changed from 400 to 0.01/s, the fatigue lives of both materials, evaluated at a peak stress of 3.2 GPa, increased by more than two orders of magnitude (Sharma et al. **

(1996a,b)). The model is based on the dynamic and quasi-static microstructural damage mechanisms observed in both materials. The microstructure of ABP and CBP silicon nitrides is modeled as a simple composite in which silicon nitride grains are embedded in a continuous network of the grain boundary phase. Since the subsurface fatigue cracks in both materials nucleate mainly from the contact region between silicon nitride grains, contact stresses between adjacent silicon nitride grains are obtained, and the frequency dependence of the fatigue lives of ABP and CBP silicon nitrides is explained on the basis of the strain-rate sensitivity of the grain boundary phase.

Ó 1998 Elsevier Science Ltd. All rights reserved. 1. Introduction In recent work by the authors (Sharma et al. (1996a,b)), the results of an experimental investigation of the eects of the grain boundary phase on the dynamic and quasi-static compression fatigue life of hot-pressed silicon nitrides are presented. The compression fatigue lives of amorphous grain boundary phase (ABP) and crystalline grain boundary phase (CBP) silicon nitrides are evaluated at strain-rates of 0.01, 0.1 and 400/s. Table 1 summarizes the results of the experiments. ABP silicon nitride was ¯uxed with 6 wt% Y2O3 and 3 wt% Al2O3, whereas CBP silicon nitride was ¯uxed with 8 wt% Y2O3 and 1 wt% Al2O3.

At a strainrate of 400/s, the fatigue life of ABP silicon nitride (104 cycles) is observed to be superior to the fatigue life of CBP silicon nitride (44 cycles). When the strain-rate is decreased from 400 to 0.01/s, the fatigue lives of both materials increases by more than two orders of magnitude and the dierence in the fatigue life of ABP silicon nitride (14,000 cycles) and CBP silicon nitride (12,000 cycles) was found to be relatively less signi®cant. The observed signi®cant dierences in the fatigue lives between 400 and 0.01/s strain-rates was accredited to the dierences in the energy loss, which is given by the enclosed area within the axial stress±strain curve, in a typical compression fatigue cycle.

The energy loss per cycle, in samples from both materials, at a strain-rate of 0.01/s was observed to be Mechanics of Materials 29 (1998) 253±273 * Corresponding author. E-mail: ceam@ames.ucsd.edu. 0167-6636/98/$ ± see front matter Ó 1998 Elsevier Science Ltd. All rights reserved. PII: 6

insigni®cant compared to the energy loss in a typical fatigue cycle at 400/s. For ABP and CBP silicon nitrides, the microcracks and dislocations were observed to nucleate mainly from the contact region between two silicon nitride grains. The grains of silicon nitride are generally separated by a grain boundary phase which can be as thin as 1±8 nm (Ahn and Thomas, 1983). For the purpose of numerical analysis, the microstructure of ABP and CBP silicon nitrides is modeled as a composite in which silicon nitride grains are surrounded by a thin boundary phase layer.

When a ceramic is subjected to compression loading, local shear stresses may act on the face of pre-existing ¯aws.

**The shear stress acting on the ¯aws causes the cracks to grow along the applied compression direction under a local tensile ®eld (Nemat-Nasser and Horii, 1982; Horii and Nemat-Nasser, 1986; Ashby and Hallam, 1986). To ®nd the critical sites where fatigue cracks are likely to nucleate, the maximum in-plane shear stress, in the vicinity of contact region, is found by varying the contact radius and the thickness of the intergranular layer.**

The eect of high pressure on amorphous silica was studied by Bridgeman and Simon (1953). They observed that amorphous silica undergoes plastic deformation at pressures of the order of 1 to 10 GPa. Since silica is present in the grain boundary phases, and very high stresses are generated at the contact regions, the grain boundary phases are assumed to have strain-rate sensitive plasticity. The strain-rate dependence of fatigue life is numerically modeled based on the strain-rate sensitivity of the grain boundary phases, and the manner by which the forces are transmitted over the contact area between adjacent grains.

In other words, the change in the maximum in-plane shear stress is examined by changing the yield strength of the grain boundary phases to mimic the behavior of a strainrate sensitive material.

In order to ®nd the elastic constants of amorphous and crystalline grain boundary phases, an attempt was made to produce these materials from appropriate oxide powders. However, the attempt was not very successful due to the lack of proper facilities. Thus, the average elastic properties of the amorphous grain boundary phase, silicon nitride grains and the crystalline grain boundary phase are estimated theoretically. These properties are then used to ®nd the contact stresses as a function of the contact radius and the thickness of the grain boundary phase.

2. Estimation of elastic properties of silicon nitride grains and amorphous and crystalline grain boundary phase To evaluate the properties of grain boundary phases, it is important to know their composition.

The composition of each grain boundary phase depends upon the relative amounts of sintering aids, as well as upon the impurity content, concentration of silica present on silicon nitride particles, and other factors. Normally, the concentration of oxygen in submicron silicon nitride particles varies from 1±3 wt%. If oxygen were to be present only in the form of silica, then the concentration of silica in silicon nitride particles varies from about 2±6 wt%. In estimating the elastic constants, the concentration of silica in silicon nitride powder is taken to be slightly under 3.5 wt%, which corresponds to 3 wt% silica in ABP and CBP silicon nitrides.

Thus, the composition of the ABP silicon nitride is taken to be: 88 wt% Si3N4, 3 wt% SiO2, 6 wt% Y2O3, and 3 wt% Al2O3, whereas the composition of the CBP silicon nitride is taken to be: 88 wt% Si3N4, 3 wt% SiO2, 8 wt% Y2O3, and 1 wt% Al2O3. In reality, some of silicon nitride is also present in the grain boundary phase, which is neglected here in the estimation of the properties of intergranular phases and silicon nitride grains. Small additions of silicon nitride to the intergranTable 1 Variation in compression fatigue lives of ABP and CBP silicon nitrides as a function of strain rate.

**Strain rate ABP silicon nitride CBP silicon nitride 400/sec 104 cycles 44 cycles 400/sec 91 cycles 33 cycles 0.1/sec 9500 cycles 3500 cycles 0.01/sec 14030 cycles 11965 cycles 0.01/sec 12150 cycles 10210 cycles 254 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273**

ular phase increase the hardness and modulus of the grain boundary phase. Thus, the estimated moduli of the crystalline and amorphous grain boundary phase are expected to be lower than the actual moduli. 2.1. Estimate of the elastic properties of amorphous grain boundary phase The elastic properties of certain oxide glasses were calculated from their chemical composition by Mackishima and Mackenzie (1973, 1975).

Their calculation was based on the consideration of the packing density and the dissociation energy of the oxide constituents per unit volume. According to them, the Young modulus of an oxide glass is given by E 83:6Vt X n i1 GiXi; 1 where Gi is the dissociation energy per unit volume of component i, Xi is the mole fraction of the ith component, and Vt is the packing density. In Eq. (1), if G is measured in kcal/cm3 then the Young modulus has the units of kbar The packing density is given by Vt i1 ViXi; 2 where M is the eective molecular weight, q is the density of the glass, and Vi is the packing factor for component i.

Table 2 lists the values of the dissociation energy per unit volume and the packing factor for SiO2, Y2O3, and Al2O3.

For 50 wt% Y2O3 + 25 wt% SiO2 + 25 wt% Al2O3 (amorphous grain boundary phase), the effective molecular weight 113.28, density 3.55 gm/cm3 , and the mole fraction of yttria, alumina, and silica are 25.1%, 27.8% and 47.1%, respectively. Substituting these values into Eqs. (1) and (2), and using the constants from Table 2, we ®nd the Young's modulus of the glassy phase to be equal to 101.2 GPa. According to Mackishima and Mackenzie (1975), the shear modulus (l) of a glass is given by l 300:96V 2 t 10:8Vt ÿ 1 X n i1 GiXi: 3 Substituting the values of the packing factor, the dissociation energy per unit volume, and the mole fraction of each component (obtained from the calculation of Young's modulus) in Eq.

(3), we obtain the shear modulus of glass as 40 GPa. Once the Young and shear moduli of the amorphous grain boundary phase are known, other elastic properties can be estimated, assuming isotropy. Table 3 lists these estimated properties of the amorphous grain boundary phase.

2.2. Estimate of the elastic properties of silicon nitride grains The concepts of micromechanics can be used to estimate the average elastic constants for the silicon nitride grains. Here, we shall use the so-called self-consistent method (Kroner, 1958; Budiansky, 1965; Hill, 1965). Assume that the glassy phase is present in the form of spherical inclusions in a matrix of silicon nitride grains. Alternatively, we could assume a more realistic situation in which silicon nitride grains are present in the form of Table 2 Dissociation energy per unit volume and packing factor of selected oxides (from Mackishima and Mackenzie (1973)) Silica Yttria Alumina Gi(kcal/cm3 ) 15.4 17.7 32 Vi 14 24.8 21.4 Table 3 Measured mechanical properties of ABP and CBP silicon-nitrides CBP silicon-nitride (8% Y2O3,1% Al2O3) ABP silicon-nitride (6% Y2O3,3% Al2O3) Young's modulus 319 GPa 304 GPa Shear modulus 126.2 GPa 120.7 GPa Poisson's ratio 0.264 0.259 Density 3248 kg/m3 3233 kg/m3 V.

Sharma et al. / Mechanics of Materials 29 (1998) 253±273 255

- spherical inclusions in a matrix of the glassy phase. In the self-consistent method, the roles of the two phases are interchangeable and the elastic constants, estimated by self-consistent method, are not aected by this choice. If the matrix and inclusions are assumed to be linearly elastic and isotropic, then the elastic constants of silicon nitride grains can be estimated either by a dilute distribution scheme in which the interaction between inclusions is neglected, or by the self-consistent scheme which accounts to some extent for the interaction between grains. Since the volume fraction of the glassy phase is greater than 10%, the self-consistent scheme is used to estimate the average elastic constants for silicon nitride grains. According to this scheme, the elastic constants of the composite material (grains and grain boundary phase) are related to the elastic constants of the inclusions and the matrix through the following relations (Nemat-Nasser and Hori, 1993): KI K K ÿ KI K K ÿ KI ÿ s1 x1a
- ÿ1 ; 4 lI l l ÿ lI l l ÿ lI ÿ s2 x1a
- ÿ1 ; 5 where f is the volume fraction of inclusions (glassy phase), and K; l; K; l; KI , and lI are the bulk and shear moduli of the matrix, composite, and inclusions, respectively. s1 and s2 are the components of Eshelby's tensor for spherical inclusions, given by, s1 1 m 3 1 ÿ m ; 6 s2 2 4 ÿ 5m 15 1 ÿ m ; 7 where m is Poisson's ratio of the composite (ABP silicon nitride).

The elastic constants of ABP and CBP silicon nitrides were calculated by measuring the pulse echo sound speed in the longitudinal and shear modes. Table 3 (Sharma et al., 1994) lists the measured elastic constants of ABP and CBP silicon nitrides. By knowing the elastic constants of ABP silicon nitride (composite) and glassy phase (inclusion), Eqs. (4) and (5) can be solved for bulk and shear moduli of silicon nitride grains. The estimated values of the aggregate properties of silicon nitride grains are listed in Table 4. 2.3. Estimate of the elastic constants of crystalline grain boundary phase Since the properties of CBP silicon nitride (composite) and silicon nitride grains (matrix) are known, Eqs.

(4) and (5) can be used to estimate the properties of the crystalline grain boundary phase (inclusion). The elastic constants of the crystalline grain boundary phase are listed in Table 4. It can be observed from Tables 3 and 4 that while most of the properties of ABP and CBP silicon nitrides fall between the properties of silicon nitride grains and amorphous/crystalline grain boundary phase, the Poisson ratio of ABP silicon nitride is lower than the Poisson ratio of silicon nitride grains and the glassy phase. This is due to the self-consistent model used to determine the properties of silicon nitride grains from the properties of ABP silicon nitride and the glassy phase.

This model ensures that the modulus of the composite falls between the modulus of the matrix and the inclusion. Since Poisson's ratio is a dimensionless number, it is not constrained by the properties of the inclusions and the matrix under the self-consistent scheme.

Table 4 Estimated elastic properties of amorphous boundary phase, silicon-nitride grains, and crystalline boundary phase ABP Silicon-nitride CBP Young's modulus 101.2 GPa 345.6 GPa 162.6 GPa Shear modulus 40 GPa 137 GPa 62.8 GPa Poisson's ratio 0.264 0.261 0.295 Bulk modulus 71.4 GPa 241 GPa 132 GPa 256 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

3. Modeling the frequency dependence of fatigue lives of ABP and CBP silicon nitrides In this section, the frequency dependence of fatigue lives of ABP and CBP silicon nitrides is modeled based on the strain-rate sensitivity of the amorphous and crystalline grain boundary phases.

Since fatigue cracks in ABP and CBP silicon nitrides initiate from contact regions between two grains, the contact stresses between adjacent silicon nitride grains, with a thin intergranular layer in between, are calculated numerically. The lattice image of three grains of silicon nitride and the grain boundary phase for ABP and CBP silicon nitrides is shown in Fig. 1(a) and (b), respectively (Sharma, 1994; Sharma et al., 1998). A thin amorphous layer is observed between crystalline grain boundary phase and silicon Fig. 1. TEM lattice image of silicon nitride showing (a) amorphous nature of grain boundary phase and (b) partial crystalline nature of grain boundary phase.

V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 257

nitride grains in CBP material in Fig. 1(b), likely due to partial crystallization of crystalline grain boundary phase. The microstructure of CBP silicon nitride, at a somewhat lower magni®cation, is shown in Fig. 2 (Sharma et al., 1994). Similar microstructure was observed for ABP silicon nitride. The microstructure of ABP and CBP silicon nitrides is rather complicated, consisting of several grain sizes and grain morphologies, which makes it dicult to determine the exact state of stress within the material.

This task is further complicated by a wide range of thickness of the intergranular layer, the possible presence of a thin amorphous layer between crystalline grain boundary phase and silicon nitride grains in CBP material, the anisotropy of silicon nitride grains and the intergranular layer, the presence of dislocations, microcracks, and other factors. For the purpose of obtaining a rough estimate of the contact stress between two impinging grains, the actual microstructure is modeled as a simple two-dimensional periodic microstructure consisting of circular and hexagonal grains with a thin intergranular layer between grains.

Due to the inability to measure the mechanical properties of the thin amorphous layer present between silicon nitride grains and the crystallized grain boundary phase in the CBP material, the grain boundary phase for the CBP material is assumed to be completely crystalline in the present model.

The idealized microstructure of the material is shown in Fig. 3. The periodically distributed unit cell is made up of two hexagonal and two circular grains (shown by dashed lines in Fig. 1). The eect of the contact radius and the thickness of the intergranular phase on the contact stresses was evaluated by generating dierent repetitive cells. Contact stresses were evaluated for six dierent contact radii (5, 10, 20, 50, 100, 250 nm) and for each contact radius, two dierent thickness (1, 5 nm) were chosen. The lateral dimension of the repetitive cell was kept constant (510 nm) and the axial dimension was varied depending upon the contact radius Fig.

2. TEM micrograph showing the microstructure of CBP silicon nitride.

Fig. 3. Idealized periodic microstructure of ABP and CBP silicon nitrides; this microstructure is used for estimating the contact stresses as functions of the contact radius and the thickness of the intergranular phase. 258 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

and thickness of the intergranular phase between hexagonal grains. The distance between parallel sides of the hexagonal grains was kept constant at 500 nm. The area fraction of the grain boundary phase was set at about 11%, by varying the diameter of the circular grains. Dierent meshes for ®nite element analysis were generated by MAZE (Hallquist, 1983) which is an input generator for the actual ®nite element code.

Fig. 4 shows a typical repetitive cell. There are about 5500 elements in each mesh; the actual number increases as the thickness of the intergranular layer is increased. When the contact radius of the hexagonal grains is equal to 250 nm, the hexagonal grains collapse into circular grains. Fig. 5 shows a repetitive cell for a contact radius of 250 nm. The average elastic constants of the repetitive cell are the same as those of ABP/CBP silicon nitride. However, the elastic constants vary widely within the plane of the repetitive cell. As a result, Fig. 4. Schematic diagram of a typical mesh used to analyze contact stresses between two grains with a thin intergranular layer between them.

V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 259

the pressure boundary condition does not give rise to uniform displacements. To achieve uniform boundary displacements (a more realistic situation), the displacement boundary conditions were speci®ed on all four sides of the repetitive cell. The axial displacements on the boundaries were speci®ed according to dlaxial rzzlaxial/E, where laxial is the axial length of the repetitive cell, rzz is the peak applied stress (3.2 GPa) used in the fatigue experiments (Sharma et al., 1996a,b), and E is the Young's modulus of the ABP/CBP silicon nitride.

The lateral displacement was speci®ed according to the relation dllateral mrzzllateral/E, where m is the Poisson ratio of ABP/CBP silicon nitride and llateral is the lateral dimension of the repetitive cell (510 nm).

The contact problem was analyzed using NIKE2D (Hallquist, 1979, 1986). NIKE2D is an implicit ®nite element code for analyzing the ®nite deformation, static, and dynamic response of twodimensional axisymmetric, plane strain and plane stress solids. All calculations were performed for the plane strain geometry. We point out again that this gives only a rough estimate of the stress state, Fig. 5. Typical ®nite-element mesh for a contact radius of 250 nm; each unit cell involves approximately 5500 elements. 260 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

- as the actual situation is neither two-dimensional nor periodic. The elastic constants for crystalline and amorphous grain boundary phases and silicon nitride grains, estimated in the previous section, were used as an input to NIKE2D. The output of NIKE2D was used in ORION (Hallquist and Levatin, 1985), which is a post-processor for NIKE2D, to ®nd the contact stresses. Once the stress tensor within each element is known, the maximum inplane shear stress {(syz)max} was found from the following relation: syzmax rzz ÿ ryy 2 n o2 s2 yz r ; 8 where rzz is the axial stress, ryy is the lateral stress and syz is the shear stress within an element. 4. Upper and lower bounds on the elastic moduli based on the periodic microstructure Bounds on the overall elastic moduli of a periodic microstructure can be found by homogenizing the microstructure and minimizing the strain energy and complementary strain energy of the homogenized microstructure (Nemat-Nasser et al., 1982; Nemat-Nasser and Hori, 1993). The microstructure can be homogenized by choosing an arbitrary reference material and by prescribing suitable eigenstrain (eigenstress) ®elds to accommodate the material mismatch. If the matrix is stier than the inclusion, then the upper bound is obtained by choosing the reference material to be the same as the matrix material, and the lower bound is obtained when the reference material is chosen as the inclusion material. For a two-phase composite material, the upper and lower bounds on the elastic moduli are given by (Nemat-Nasser and Hori, 1993; Nemat-Nasser et al., 1993), C CM fX CX ÿ CM ÿ1 fXCXX CM h iÿ1 ; 9 C ÿ CX 1 ÿ fX CM ÿ CX ÿ1 fX CXX CX
- ÿ1 ; 10 where fX is the volume fraction of inclusions, CM and CX are the elasticity tensor for matrix and inclusions, respectively, and CXX is the function of the reference elasticity tensor and the geometry of the inclusion.
- Universal upper and lower bounds can be obtained based on only the volume fraction of the inclusions, without considering the geometry of the inclusion in the calculation of CXX . The CXX matrix in this case is given by the following relations (Nemat-Nasser and Hori, 1993): fXCXX iijj 1 ÿ fX 1 ÿ 2m 2l 1 ÿ m ; 11a fXCXX ijij 1 ÿ fX 3 ÿ 4m 2l 1 ÿ m ; 11b where l is the shear modulus and m is Poisson's ratio of the reference material. For an isotropic material, the two-dimensional stiness matrix for plane strain geometry is given by E 1 ÿ m 1 m 1 ÿ 2m Em 1 m 1 ÿ 2m Em 1 m 1 ÿ 2m E 1 ÿ m 1 m 1 ÿ 2m m ; 12 where E is the Young modulus of the reference material. The elasticity tensor for the matrix and the inclusion can be obtained by substituting E and n into the above equation. Substituting CM , CX , and Eq. (12) into Eqs. (9) and (10), the universal upper and lower bounds are found as, C U 540:12 282:68 0:0000 282:68 540:12 0:0000 0:0000 0:0000 334:80 ; 13a C ÿ U 374:71 117:28 0:0000 117:28 374:71 0:0000 0:0000 0:0000 223:84 ; 13b If the geometry of the inclusion is also accounted for in the determination of the bounds, then CXX is given by the following relation: CXX X
- 1 n gX ÿngX n^ C n; C: 14 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 261

- In Eq. (14) the term associated with ni.ni 0 is excluded from the summation (ni nip/ai, i 1, 2, i not summed; where ni is an integer; and ai is the dimension of the unit cell in the ith direction). The eect of the inclusion geometry is fully accounted for in the g-integral de®ned by g n 1 VXX Z exp in:x dx: 15 For an isotropic material, ^ C n; C is given by the following relation: ^ C n; C 1 l sym n 1 2 n x1a m 16 where n n=jnj n= n:n p : The lower and upper bounds on the elastic moduli can be found by substituting Eq. (14) into Eqs. (9) and (10). To this end, the intergranular phase (inclusion) of the unit cell shown in Fig. 2 was divided into approximately 1200 elements. To calculate the g-integral, each of the 1200 elements was approximated by a square. The term involving the geometry of the inclusions, given by Eq. (14), is evaluated for two square elements Xr and Xs with dimensions lr and ls and with centers at xr 0 and xs 0, respectively. The result is, gX ngX ÿn cosfn
- xr 0 ÿ xs 0g 16 sin n1lr=2 sin n2lr=2 sin n1ls=2 sin n2ls=2 n2 1n2 2l2 r l2 s ( ) : 17 Substituting Eqs. (17) and (16) into Eq. (14), CXX can be calculated numerically when the reference material is chosen to be either the matrix or the inclusion. Since the series in Eq. (14) converges rather fast, n1 and n2 were varied from )50 to +50. Once CXX is known, the upper and lower bounds on the elastic moduli can be obtained from Eqs. (9) and (10). This gives, C 399:68 143:77 0:0000 143:77 399:68 0:0000 0:0000 0:0000 258:11 ; 18a Cÿ 399:10 144:36 0:0000 144:36 399:10 0:0000 0:0000 0:0000 258:82 : 18b The upper and lower bounds are essentially the same (the dierence between any two elements being less than 0.4% which is within the numerical errors). These bounds lie between the universal bounds. For a composite having a periodic microstructure, these bounds give a better estimate of the overall properties compared to the dilute distribution and self-consistent schemes.

Contact stresses were found for two dierent cases: (a) elastic silicon nitride grains and elastic grain boundary phases, and (b) elastic silicon nitride grains and strain-rate sensitive grain boundary phases. 5. Elastic silicon nitride grains, elastic grain boundary phase In order to ®nd the critical sites within the microstructure where fatigue cracks are likely to initiate, the maximum in-plane shear stress between contacting grains is calculated as a function of the contact radius and the thickness of the intergranular layer. Fig. 6 ((a) and (b)) show the variation of the maximum in-plane shear stress on the surface of the silicon nitride grains for CBP silicon nitride, for 1 and 5 nm thickness of the intergranular layer, respectively.

The abscissa of these ®gures represents the distance along the surface of the grain (measured from the contact point) normalized by (2pR/360), where R is the contact radius. In other words, the points on the surface of the hexagonal grains are represented by an angle that is measured counterclockwise from the contact point.

When the thickness of the intergranular layer is small (1 nm), then the maximum in-plane shear stress does not occur at the contact point (h 0), but at a distance from it. As the thickness is increased, the maximum in-plane shear stress occurs at the contact point for grains with contact radius less than or comparable to the thickness of the intergranular layer. For a ®xed contact radius, a slight increase in the maximum in-plane shear stress with increasing intergranular thickness, was 262 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

observed.

This increase is probably due to the relaxation of the lateral constraint which decreases the lateral stress (ryy) at a faster rate than the normal axial stress (rzz). Thus, according to Eq. (8), the maximum in-plane shear stress increases slightly. Thus, the change in the maximum in-plane shear stress depends upon the contact radius and the thickness of the intergranular layer. For a given constant thickness, the maximum in-plane shear stress decreases as the contact radius Fig. 6. Variation of the maximum in-plane shear stress on the surface of contacting grains for CBP silicon-nitride at (a) 1 nm, and (b) 5 nm thickness of crystalline grain boundary phase.

V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 263

is increased to 100 nm. However, the maximum inplane shear stress for a contact radius of 250 nm is greater than that for 50 nm and 100 nm contact radii at 1 and 5 nm intergranular layer thickness. For a contact radius of 250 nm, the grain boundary phase is more uniformly distributed (along the y-axis) compared to 50 and 100 nm contact radii. For a ®xed lateral displacement, as the concentration of the soft phase along the y-axis, in the vicinity of contact region increases, the lateral constraint (ryy) increases.

An increase in the lateral constraint decreases the maximum in-plane shear stress, according to Eq. (8). In fact, if the elastic properties of the circular grains are chosen to be the same as those of the grain boundary phase, then the maximum in-plane shear stress decreases considerably, likely due to a greater lateral constraint. The diameter of the circular grains also affects the maximum in-plane shear stress. The maximum in-plane shear stress increases as the diameter of the circular grains increases. Thus, for a contact radius of 250 nm (smaller concentration of soft phase along the y-axis around the contact region), the maximum in-plane shear stress is greater than that for a contact radius of 100 nm.

Fig. 7 ((a) and (b)) show the variation of the maximum in-plane shear stress for ABP silicon nitride for 1 and 5 nm thickness of the glassy phase. Similarly to CBP silicon nitride, a slight increase in the maximum in-plane shear stress with increasing grain boundary phase thickness was observed for a constant contact radius. It is interesting to note that the maximum in-plane shear stress for a contact radius of 250 nm is less than the corresponding stress for a contact radius of 100 nm for 1 and 5 nm intergranular layer thickness. Thus, in addition to the contact radius, the thickness of the intergranular layer, and the manner in which the grain boundary phase is distributed, the maximum in-plane shear stress also depends upon the elastic properties of the grains and the grain boundary phase.

For equivalent repetitive cells, the maximum inplane shear stress for ABP silicon nitride is greater than the corresponding stress for CBP silicon nitride. For small thickness of the intergranular phase between silicon nitride grains, the contact stresses depend upon the relative mismatch in the elastic properties between the grains and the grain boundary phase. As an extreme case, if the elastic properties of the grains are the same as those of the grain boundary phase, then rzz is the same everywhere and ryy is zero. Thus, higher contact stresses in ABP silicon nitride compared to CBP silicon nitride, are due to higher relative mismatch between the glassy phase and silicon nitride grains in the ABP material.

- 6. Elastic silicon nitride grains, elastic±plastic grain boundary phase In this section, the eect of strain-rate sensitivity of the grain boundary phase on the maximum in-plane shear stress is examined. A repetitive cell with a contact radius of 50 nm and an intergranular thickness of 5 nm was chosen for purposes of analysis. The strain-rate sensitive behavior of a material may be expressed by an equation of the type, r rY 1 e e0
- n _ e _ e0 !m ; 19 where rY is the yield stress, e/e0 is the ratio of the strain with respect to the reference strain, _ e=_ e0 is the ratio of the strain-rate with respect to the reference strain-rate, n is the strain hardening exponent, and m is the strain-rate sensitivity exponent. For a constant strain-rate, the above equation reduces to an equation of the type r r0 1 e=e0 n , where r0 is a constant. This equation reduces to an elastic-perfectly plastic equation for n 0. For n 1, we obtain a bilinear stress±strain relation. Thus, as a particular case, the strain-rate sensitive behavior can be modeled by changing the yield stress for an elastic-plastic material with isotropic linear hardening. In a typical fatigue test, the macroscopic applied loading rate is constant. For ABP and CBP silicon nitrides a constant loading rate gives rise to a constant macroscopic applied strain-rate. The local strain-rate within the highly heterogeneous microstructure of ABP and CBP silicon nitrides is not constant. The present approach is based on the Taylor model (Taylor, 1934) which assumes that the local strain-rate is the same 264 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

as the overall strain-rate. Thus, the in-plane shear stress is obtained assuming that the local strain-rate is the same as the macroscopic applied strain-rate which is a constant. The model can be re®ned to take care of the local strain-rates to explain the dierences in the strain-rate dependence of the fatigue life of silicon nitride, using a concentration tensor (Nemat-Nasser and Hori, 1993), but Fig. 7. Variation of the maximum in-plane shear stress on the surface of contacting grains for ABP silicon-nitride at (a) 1 nm, and (b) 5 nm thickness of amorphous grain boundary phase.

Sharma et al. / Mechanics of Materials 29 (1998) 253±273 265

for the present purposes, it is felt that the Tylor model is adequate. The elastic-plastic behavior will thus be represented by the following equation: rY r0 EPeP ; 20 where r0 is the initial eective yield stress, rY is the current eective yield stress, eP is the eective plastic strain, and EP is the hardening modulus (slope of yield stress-eective plastic strain curve). The eective stress in the intergranular layer, in the vicinity of a contact point, was evaluated by assuming isotropic and linearly elastic silicon nitride grains and an elastic-perfectly plastic grain boundary phase.

The eect of the yield stress on the maximum in-plane shear stress was evaluated for elastic silicon nitride grains and the elasticplastic grain boundary phase. Fig. 8 shows the effect of changing the yield stress on the maximum in-plane shear stress for CBP silicon nitride. For elastic silicon nitride grains and the elastic intergranular phase (curve labeled elas, 346 from Fig. 7), the maximum eective stress in the intergranular layer, in the vicinity of the contact region, was about 3 GPa. The maximum in-plane shear stress decreases monotonically as the eective yield stress is decreased.

The decrease in the maximum in-plane shear stress is about 14% when the eective yield stress decreases from 3 to 2 GPa. Thus, as the strain-rate (eective yield stress of the intergranular layer) is increased, the maximum in-plane shear stress at the contact region increases, thereby increasing the fatigue crack nucleation sites and the growth of fatigue cracks. In other words, as the strain-rate is increased, the fatigue life of CBP silicon nitride decreases.

The variation of the maximum in-plane shear stress with respect to the eective yield stress of the intergranular layer, for ABP silicon nitride, is shown in Fig. 9. A slight increase (about 1.1%) in the maximum in-plane shear stress is observed when the eective yield stress decreases from 3.6 (elastic silicon nitride grains, elastic glassy phase) to 3.0 GPa. The relative change in the maximum in-plane shear stress with respect to the yield stress of the intergranular phase, is substantially less in ABP silicon nitride than in CBP silicon nitride.

The eect of the hardening modulus on the maximum in-plane shear stress, for ABP and Fig.

8. Variation of the maximum in-plane shear stress, on the surface of contacting grains, with respect to the yield stress of the crystalline grain boundary phase. 266 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

CBP silicon nitrides, is shown in Fig. 10(a) and (b), respectively. The eective yield stress of the intergranular phase was taken as 2.5 GPa. The hardening modulus of the crystalline phase was chosen as 0 (elastic-perfectly plastic phase), 30, 80, and 120 GPa, whereas the hardening modulus of the glassy phase was chosen as 0 (elastic-perfectly plastic glassy phase), 20, 50, and 80 GPa. As the hardening modulus increases, the maximum inplane shear stress increases. The increase in the maximum in-plane shear stress with respect to the hardening modulus is relatively less in ABP silicon nitride compared to that in CBP silicon nitride.

It was mentioned earlier that a plane strain geometry of the repetitive cell is used to analyze the contact problem. The preclusion of the out-ofplane movement of the repetitive cell, under plane strain geometry, results in a high lateral constraint which lowers the maximum in-plane shear stress. In reality, out-of-plane movement is allowed to some extent. Thus, the actual values of the maximum in-plane shear stress should be lower than those shown in Figs. 8 and 9, and 10. To ®nd the change in the maximum in-plane shear stress when the contact between grains occurs at an angle to the applied compression, the repetitive unit cell (see Fig.

4) was modi®ed slightly. The diameter of the circular grains on the side of the cell was made equal to the diameter of the grains at the top and bottom of the cell (250 nm). The axial dimension of the repetitive cell was increased to accommodate the grains on the side, whereas the radial dimension was kept constant at 505 nm. Fig. 11 shows the top half of the modi®ed repetitive cell used to ®nd the contact stress between the contacting grains. Fig. 12(a) and (b) show the variation of the maximum inplane shear stress with respect to the yield stress of the intergranular layer, on the surface of the contacting grain for ABP and CBP silicon nitrides, respectively, for a 5 nm thickness of the intergranular layer.

Unlike in previous cases, the maximum in-plane shear stress is not symmetric about the contact point. It can be observed from Figs. 8 and 9, and 12(a) and (b) that the change in the maximum in-plane shear stress with respect to the yield stress of the intergranular layer is at least three times greater for the modi®ed repetitive cell. The maximum in-plane shear stress on the surface of the contacting grains, for elastic grains and elastic glassy grain boundary phases, increases by Fig. 9. Variation of the maximum in-plane shear stress, on the surface of contacting grains, with respect to the yield stress of the amorphous grain boundary phase.

V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 267

approximately 30% (see Fig. 6(b), R 250 curve, and Fig. 12(a), topmost curve) when the grains contact each other at an angle of about 45° with respect to the applied compression direction. The corresponding increase in the maximum in-plane shear stress on the contact surface of the silicon nitride grains for CBP silicon nitride is about 40%. Thus, the fatigue cracks in ABP and CBP Fig. 10. Eect of the hardening modulus on the maximum in-plane shear stress for (a) ABP silicon nitride, and (b) CBP silicon nitride (yield stress of glassy phase 2.5 GPa, tm tangent modulus).

268 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

silicon nitrides are more likely to initiate from grains that contact each other at an angle close to 45° with respect to the applied compression direction. To summarize, the dierence in the fatigue lives (Sharma et al., 1996a,b) between quasi-static strain-rates (0.1 and 0.01/s) and dynamic strainrates (400/s) can be explained on the basis of the strain-rate sensitivity of the grain boundary phases. At high strain-rates, the maximum in-plane shear stress at the contact surface and within the grains is greater than the corresponding maximum in-plane shear stress at lower strain-rates.

The maximum in-plane shear stress depends upon the properties of the grains and the grain boundary phase, contact radius of the grains, thickness of the grain boundary phase between the contacting grains, and the way the grain boundary phase is distributed within the microstructure. Higher values of the maximum in-plane shear stress, at high Fig. 11. Typical ®nite-element mesh used to estimate the contact stress when the grains contact each other at an angle to the applied compression direction.

V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 269

strain-rates, results in a greater number of initiation sites for fatigue cracks, and higher fatigue crack growth rates per cycle. 7. Discussion Based on the simpli®ed microstructure of silicon nitride, it has been shown that the fatigue lives Fig. 12. Variation of the maximum in-plane shear stress, on the surface of contacting grains, with respect to the yield stress of (a) amorphous, and (b) crystalline grain boundary phases. 270 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

of ABP and CBP silicon nitrides depend upon the fatigue frequency if the intergranular phase is strain-rate sensitive.

As mentioned earlier, the actual microstructure of both materials is rather complicated, and it is not possible to model the exact microstructures of ABP and CBP silicon nitrides. Thus, the model presented in this investigation does not explain the observed dierences in the behavior of ABP and CBP silicon nitrides. The explanation of the dierences in the behavior of ABP and CBP silicon nitrides requires a better understanding of the contact stress as a function of the loading rate. In addition to the contact radius, the thickness and distribution of the intergranular layer, and the elastic properties of the grains and the grain boundary phase, the contact stress between impinging silicon nitride grains also depends upon the internal stresses within the material and the variation of the yield stress and hardening parameter of the grain boundary phase as a function of strain-rate.

The actual contact stress between silicon nitride grains can be higher or lower in the ABP or CBP materials, depending upon the internal stress and strain-rate sensitivity of the boundary phase. For similar internal stress and strain-rate sensitive behaviors of both materials, higher fatigue life can be observed for the material that experiences higher contact stress due to the dierences in the fatigue crack propagation rates. The propagation of fatigue cracks depends upon the strength of the boundary phase, the interfacial strength between silicon nitride grains and the boundary phase, etc.

Thus, modeling of the dierent behaviors of ABP and CBP silicon nitrides is rather complex, as it requires detailed knowledge about silicon nitride grains, the boundary phase, the internal stresses, etc.

The change in the peak stress for two orders of magnitude dierence in the fatigue life can be estimated and compared with the numerical results. Let us assume that the growth of microcracks per cycle is governed by the Paris equation (Paris et al., 1961) da=dN A DK n . According to this equation, the dierence in the crack growth rate depends upon the crack velocity parameter (n), and the dierence between the maximum and the minimum stress intensity factor (DK). The crack velocity parameter has been obtained experimentally for dierent types of silicon nitrides. Ko (1987) obtained a value of 25 for sintered silicon nitride (rotary bending fatigue), Matsuo et al.

(1983) obtained a value of 55 and 63 for sintered and hot-pressed silicon nitrides (under positive cut sinusoidal cycle), respectively, and Nikkila and Mantyla (1989) observed values of 31 and 41 for two dierent types of sintered silicon nitrides and a value of 43 for hot-pressed silicon nitride (under tension-compression loading) as the crack velocity parameter. If the crack velocity parameter for ABP and CBP silicon nitrides is chosen as 40, then the crack growth rate decreases by two orders of magnitude for every 9% decrease in the peak stress. The change in the maximum in-plane shear stress (see Figs.

8 and 9) on the surface of the contacting grains is of this order of magnitude. However, away from the contact region, the change in the stress components become negligible as the strain-rate is changed. Based on this argument, the actual change in the peak stress to cause two orders of magnitude dierence in the fatigue life is more than 9%. On the other hand, the number of cracks generated in ABP and CBP silicon nitrides, per cycle, increases as the strain-rate is increased from 0.01 to 400/s. Consequently, the eective crack growth rate (crack growth rate assuming the same number of microcracks) is greater at 400/s compared to that at 0.01/s.

Thus, the actual change in the peak stress for two orders of magnitude dierence in the fatigue life is less than the predicted change based on the Paris equation. Regardless of the process that dominates the eective crack growth rate, the actual change in the peak stress is not expected to deviate much from the predicted change.

Based on the observation of Bridgeman and Simon (1953), the grain boundary phase was assumed to have strain-rate sensitive plasticity, whereas silicon nitride grains were assumed to be elastic. If one assumes silicon nitride grains to have strain-rate sensitive plasticity and the grain boundary phase to be elastic, then it is observed that, compared to the change in the yield stress of silicon nitride grains has a much more profound eect on the corresponding change in the maximum V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 271

in-plane shear stress.

This is likely due to high volume fraction of silicon nitride grains (89%). Finally, the hysteresis in the stress-axial strain curves for both materials at dynamic strain-rates (Sharma et al., 1996a,b) can be explained on the basis of the energy dissipation processes occurring within the materials. The two dominant processes that result in a loss of energy within the materials are the generation and propagation of microcracks, and the plastic deformation of the grain boundary phase. Since the volume fraction of the grain boundary phase is small (approximately 11%) and the plasticity of the intergranular phases is assumed to occur in the vicinity of the contacting grains, the plasticity of the grain boundary phase does not consume much energy.

At high strain-rates, the initiation of a large number of fatigue cracks and higher crack growth rates results in the loss of a large amount of energy within the materials. Consequently, the opening of the stress-axial strain curve is signi®cant at dynamic strain-rates compared to that at the quasi-static strain-rates.

8. Conclusions The contact region between two silicon nitride grains was identi®ed as the fatigue crack nucleation site in ABP and CBP silicon nitrides, at 0.01 and 400/s strain-rates. The degradation of the dynamic fatigue life compared to the quasistatic fatigue life is explained on the basis of the strain-rate sensitivity of the grain boundary phase and/or silicon nitride grains, and the manner by which the forces are transmitted over the contact area of the contacting grains. The microstructure of the materials was modeled as a periodic microstructure and the contact stresses between adjacent silicon nitride grains were calculated numerically.

It was observed that, at low strain-rates, the grain boundary phase and/or silicon nitride grains yield at a lower stress, thereby decreasing the contact stress, the average stress, and more importantly, the maximum shear stress in silicon nitride grains. This results in lower dislocation activity and lower crack-growth rates, and consequently the fatigue lives of ABP and CBP silicon nitrides increase as the strain-rate is decreased from 400 to 0.01/s. Acknowledgements This research was supported by a grant from the Army Research Oce under contracts No. DAAL-03-86-K-0169 and DAAL-03-92-K-0002 to UCSD.

The computations reported in this paper were performed on a CRAY-C90 computer at the San Diego Supercomputer Center. References Ahn, C.C., Thomas, G., 1983. Microstructure and grain boundary composition of hot-pressed silicon nitride with yttria and alumina. J. Amer. Ceram. Soc. 66 (1), 14± 17.

Ashby, M.F., Hallam, S.D., 1986. The failure of brittle solids containing small cracks under compressive stress states. Acta. Meta. 34 (3), 497±510. Bridgeman, P.W., Simon, I., 1953. Eect of very high pressure on glass. J. Appl. Phys. 24, 405±413. Hallquist, J.O., 1983. MAZE ± An input generator for DYNA2D and NIKE2D. University of California, Lawrence Livermore National Laboratory, Rept. UCID - 19029. Hallquist, J.O., 1986. NIKE2D: A vectorized implicit, ®nite deformation, ®nite element code for analyzing the static and dynamic response of 2-D solids with interactive rezoning and graphics.

University of California, Lawrence Livermore National Laboratory, Rept. UCID-19677.

Hallquist, J.O., 1979. NIKE2D: An implicit, ®nite deformation. Finite element code for analyzing the static and dynamic response of two-dimensional solids. University of California, Lawrence Livermore National Laboratory, Rept. UCRL-52678. Hallquist, J.O., Levatin, J.L., 1985. ORION: An interactive color post-processor for two dimensional ®nite element codes. University of California, Lawrence Livermore National Laboratory, Rept. UCRL-19310. Horii, H., Nemat-Nasser, S., 1986. Brittle failure in compression: Splitting, faulting and brittle-ductile transition. Phil. Trans. Roy. Soc. Lond. 319 (1986), 337±374.

Ko, H.N., 1987. Fatigue strength of sintered silicon nitride under rotary bending. J. Mat. Sci. Lett. 6, 175±177. Makishima, A., Mackenzie, J.D., 1975. Calculation of bulk modulus, shear modulus and poisson's ratio of glass. J. Non-Cryst. Solids 17, 147±157.

Makishima, A., Mackenzie, J.D., 1973. Direct calculation of Young's modulus of glass. J. Non-Cryst. Solids 12, 35± 45. Matsuo, Y., Hattori, Y., Katayama, Y., Fukuura, I., 1983. Cyclic fatigue behavior of ceramics. In: Riley, F.L. (Ed.), Progress in Nitrogen Ceramics, pp. 515±522. Nemat-Nasser, S., Iwakuma, T., Hejazi, M., 1982. On composites with periodic structure. Mechanics of Materials 7, 239±267. 272 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273